Synthesis and Characterization of Metallopolymer Networks Featuring Triple Shape-Memory Ability Based on Different Reversible Metal Complexes

This study presents the synthesis and characterization of metallopolymer networks with a triple shape-memory ability. A covalently crosslinked polymer network featuring two different additional ligands in its side chains is synthesized via free radical polymerization (FRP). The subsequent addition of different metal salts leads to the selective formation of complexes with two different association constants (Ka), proven via isothermal titration calorimetry (ITC). Those two supramolecular crosslinks feature different activation temperatures and can act as two individual switching units enabling the fixation and recovery of two temporary shapes. The presented samples were investigated in a detailed fashion via differential scanning calorimetry (DSC), thermogravimetric analysis (TGA), and FT-Raman spectroscopy. Furthermore, thermo-mechanical analyses (TMA) revealed excellent dual and triple shape-memory abilities of the presented metallopolymer networks.


Introduction
Recently, intelligent materials have become more and more important. The use of stimulus responsive polymers can bring several advantages and improvements in many areas [1][2][3]. By combining metal complexes with polymers, it is possible to create completely new materials. In such metallopolymers, it is possible to combine the outstanding properties of both material classes, which brings enormous benefits in some areas of application and can even open the way into new ones [4]. Through the respective choice of metal ion, ligand, and the associated stability of the resulting metal complex, it is possible to control the polymer properties in a targeted manner and to adapt them to the respective requirements [5]. This new class of polymers can be used, for example, in the field of catalysis [6] or opto-electronics [7] and sensors [8]. The implementation of reversible metal-complexes into the polymeric structure makes the synthesis of stimuli-responsive materials easier. Depending on the type of metallopolymer and the utilized metal-ligand interaction, thermally [9], photo-chemically [10], mechanically [11], or redox-reaction [12] induced switching of the materials is possible. In addition to the mentioned areas of possible applications, the utilization of intelligent metallopolymers for the synthesis of polymers with self-healing [13] or shape-memory abilities [14,15] has become more and to the best of our knowledge, there are no examples for triple shape-memory polymers in which both switching units are based on two different supramolecular crosslinks.
This study presents the synthesis of supramolecular triple shape-memory polymers, in which the two switching units are formed by two metal complexes with different activation temperatures. The stable phase of the system was achieved by covalent crosslinking of the polymeric network.
Nuclear magnetic resonance (NMR) spectra were measured using a Bruker AC 250 (250 MHz), Bruker AC 300 (300 MHz), Bruker AC 400 (400 MHz), and a Bruker AC 600 (600 MHz) spectrometers (Billerica, MA, USA) at 298 K if not stated differently. The chemical shift is given in parts per million (ppm on δ Scale) related to deuterated solvent. All NMR spectra are presented in the Supplementary Information.
Elemental analysis (EA) was performed utilizing a Vario El III (Elementar, Langenselbold, Germany). All results of the elemental analyses are summarized in the Supplementary Information. For the covalently crosslinked polymers and metallopolymer networks, the calculated values are based on the ratio of the monomers utilized for the polymerization.
Isothermal titration calorimetry (ITC) measurements were performed using a standard volume Nano ITC (TA Instruments) at 303 K. The solutions were always prepared prior to use in dry solvents utilizing vacuum dried ligand and metal salt. Blank titrations in dry solvent were performed and subtracted from the corresponding titrations to remove the effect of dilution. The fitting of the measured data was performed with the NanoAnalyze program from TA instruments. The resulting titration plots are displayed in the Supplementary Information.
Size exclusion chromatography (SEC) measurements were performed on the following setup: Shimadzu with CBM-20A (system controller), DGU-14A (degasser), LC-20AD (pump), SIL-20AHT (auto sampler), CTO-10AC vp (oven), SPD-20A (UV detector), RID-10A (RI detector), PSS SDV guard/1000 Å/1,000,000 Å (5 µm particle size) chloroform/isopropanol/triethyl-amine [94/2/4] with 1 mL/ min at 40 • C, poly(methyl methacrylate) (standard). The resulting SEC curves are displayed in the Supplementary Information. Differential scanning calorimetry (DSC) was measured on a Netzsch DSC 204 F1 Phoenix instrument (Selb, Germany) under a nitrogen atmosphere with a heating rate of 20 K min −1 (first and second heating cycle) and 10 K min −1 (third heating cycle). The resulting DSC curves are displayed in the Supplementary Information. Thermogravimetric analysis (TGA) was carried out under normal atmosphere with a heating rate of 10 K min −1 using a Netzsch TG 209 F1 Iris (Selb, Germany). The resulting TGA curves are displayed in the Supplementary Information. Thermo-mechanical analyses (TMA) were performed on an MCR 301 rheometer from Anton Paar (Graz, Austria) using the convection oven device CTD 450, which covers a temperature range from −150 to 450 • C. Rectangular samples of approximately 30 mm length, 10 mm width, and a thickness ranging between 2 and 5 mm were measured using a solid rectangular fixture (SRF) designed for solid samples. After fixing the samples, a free length ranging between approximately 15.0 and 20.5 mm resulted in the experiments. All TMA measurements (dual and triple) were performed analogically to literature procedure [33,37]. All resulting TMA plots are displayed in the Supplementary Information.
FT-Raman spectroscopy measurements were performed on a Multispec Fouriertransform Raman-Spectrometer (Bruker Corporation, Billerica, Massachusetts, United States of America) in the range between 100 and 4000 cm −1 with a spectral resolution of 4 cm −1 . The Raman excitation light at 1064 nm was provided by a Nd:YAG laser (Klastech DeniCAFC-LC-3/40, Dortmund, Germany). The laser power at the sample was set to 100 mW and 512 accumulated scans were recorded for each sample to improve the signalto-noise ratio. Full spectra of all samples, including reference materials are shown in the Supplementary Information.

Synthesis of the Metallopolymer Networks
To synthesize the metallopolymer networks P1-Fe/Fe, P1-Co/Co, P1-Fe/Zn, and P1-Co/Zn, the covalently crosslinked polymer network P1 was placed in a 20 mL vial and was swollen in dichloromethane (5 mL). The calculated amount of the metal salt was separately dissolved in methanol (2 mL) and added to the swollen polymer network. In the case of the utilization of two different salts for the synthesis of P1-Fe/Zn and P1-Co/Zn, first the salt for the formation of the strong terpyridine complexes and afterwards the zinc triflate for the formation of the labile triazole-pyridine complexes was added. The resulting metallopolymer networks were dried for 24 h under vacuo at a temperature of 40 • C to remove the solvents. The utilized quantities for the synthesis are listed in Table 1.

Isothermal Titration Colorimetry
For the utilization of two different metal-complexes as two switching units in a triple shape-memory polymer, the complex association constant K α of the formed metal complexes plays an important role. In order to determine those values, as well as the stoichiometry of the formed complexes, isothermal titration calorimetry (ITC) measurements were performed with different model systems and metal salts. Based on former studies [14,18,37], it was decided to utilize 2,2 :6 ,2"-terpyridine (Tpy), known for the formation of stable complexes with higher activation temperatures with several metal salts. For the second switching unit, which should feature a lower activation temperature, a pyridine-triazole ligand (Triaz-Py) was applied. The synthesis of the Triaz-Py ligand without any polymerizable group, which was utilized as model system in the ITC investigations, was performed according to a literature procedure [35,36]. The reaction scheme is presented in the Supplementary Information (see Scheme S2). The results of the ITC measurements with the two different ligands and several salts are presented in Table 2 and Figures S1-S4. For FeSO 4 and Co(OAc) 2 , these results revealed the formation of stable complexes with terpyridine, while the complexes with triazole-pyridine are rather weak. Additionally, it was found that Zn(TFMS) 2 also forms labile complexes with the Triaz-Py, which should feature a rather low activation temperature as well. Regarding the triazole-pyridine ligand, the association constant determined for the formation of the complex with Zn(TFMS) 2 was the lowest. The highest value in this context was found with Co(OAc) 2 , while the determined value for FeSO 4 was between those two. From this, the following complex stability should be derived based on the metal salt utilized: Zn < Fe < Co. In contrast, the terpyridine complex formed with iron sulfate has a significantly higher value for K α compared to the cobalt bis-complex and should, therefore, also be significantly more stable. Table 2. Determined complex association constants (K α ) and stoichiometry (n) via isothermal titration calorimetry.

Synthesis of a Polymer Network and Metallopolymer Networks
For the synthesis of the covalent crosslinked polymer network (P1) bearing two different ligands in the side chains, the required ligand monomers, 6-(2,2 :6 2"-terpyridin-4yloxy)-hexyl methacrylate (Tpy-MA) and 11-[4-(pyridine-2-yl)-1H-1,2,3-triazol-1-yl]undecanylmethacrylate (Triaz-Py-MA), were synthesized according to literature procedures [13,35,36] (see SI Schemes S1 and S2). Subsequently, the two ligand monomers (10% of each) were polymerized via free radical polymerization together with n-butyl methacrylate (BMA) as main monomer and 5% triethyleneglycol dimethacrylate (TEGDMA) as covalent crosslinker using 2,2 -azobis(2-methylpropionitrile) (AIBN) as initiator. The schematic representation of the synthesis of P1 is displayed in Scheme 1a. The obtained polymer revealed swelling; however, it was insoluble in any common solvent (e.g., chloroform, DMF, tetrahydrofuran, or acetone) indicating the successful synthesis of a covalent crosslinked polymer network. The elemental analyses revealed a nitrogen content of 5.87%, which fits quite well with the calculated value of 5.93%. The latter value was calculated based on the utilized monomer ratios during the polymerization. For this reason, it can be assumed that the polymer network has the targeted composition. An exact determination of the composition was not possible due to the above-mentioned insolubility. For the formation of metallopolymer networks different salt combinations, based on the ITC results, were added to P1, which was swollen in chloroform. The stoichiometries determined during the ITC measurements were rounded, since a stoichiometry of 1.6 was determined for the formation of the triazole-pyridine complex with iron(II) sulfate or cobalt(II) acetate. However, literature reports also indicated the formation of 2:1 complexes [38]. For this reason, a ratio of 2 to 1 was utilized as the ratio of ligand (either triazole-pyridine or terpyridine) to metal salt. The schematic representation of the synthesis of the metallopolymer networks is presented in Scheme 1b. Iron(II) sulfate or cobalt(II) acetate as salt were used for the formation of the stronger complexes with the terpyridine ligands. Furthermore, those two salts and, additionally, zinc(II) trifluoromethane sulfonate were utilized for the formation of the weaker complexes formed by the triazole-pyridine ligands. The required amount of salt(s) was calculated based on the ligand content of P1, which was assumed to be the same as in the monomer mixture indicated by the nitrogen content found in elemental analyses. In total, four different covalently and supramolecular crosslinked metallopolymer networks P1-Fe/Fe, P1-Co/Co, P1-Fe/Zn, and P1-Co/Zn were prepared.

Raman Spectroscopic Investigations
To confirm the formation of the metal complexes inside the polymers and to investigate the binding environment, FT-Raman spectroscopy was performed on the polymer P1 and its derivatives. The Raman spectra of P1 and the metallopolymer networks P1-Fe/Fe, P1-Co/Co, P1-Fe/Zn, and P1-Co/Zn are depicted in Figure 1 (full spectra are presented in the Supplementary Information, Figure S34). Raman spectroscopy is a well-established tool to investigate active centers inside polymer environments and was already utilized in previous work to investigate terpyridine and trityl-histidine complexes of zinc, iron, and nickel ions [14,37]. Therefore, changes to the Raman spectrum of Tpy are already well known. Namely, the aromatic vibrations at 996 cm −1 , 1320 cm −1 , and 1566 cm −1 blue shift due to a conformational change of the Tpy ligand upon metal binding, causing a trans/cis isomerization [14]. To investigate the changes in the Raman spectra upon binding to the Triaz-Py inside the polymer environment of P1, model polymers of BMA functionalized with only one of the two ligands were investigated (see Figures S35 and S36). The synthesis of those model polymers and metallopolymer networks is presented in the Supplementary Information (Scheme S3). The observed changes for Triaz-Py unfortunately lie in regions similar to those relevant for Tpy. This is due to the similar chemical nature of both moieties (both are N-heteroaromatic structures), leading to overlapping bands. Nevertheless, marker bands for Triaz-Py are a characteristic blueshift of the vibrations at 980, 1550, and 1600 cm −1 upon addition of a metal salt. Interestingly, these shifts, particularly for the bands at 1550 and 1600 cm −1 are much stronger for zinc compared to cobalt and iron. Differences in coordinating behavior of zinc and iron to Triaz-Py-like ligands are known from literature and are attributed to the longer bond lengths and geometric flexibility of the d 10 Zn 2+ ion compared to the d 6 Fe 2+ [39]. Since iron and cobalt generally behave chemically similar, it is reasonable to assume that this difference is also applicable to zinc/cobalt and therefore explains the different strength of the band shifts for these ions. In the context of this work, these differences prove very helpful, since they should allow the differentiation of Zn-Triaz-Py from Co/Fe-Triaz-Py, thereby enabling ion sensitive spectroscopy in the mixed ion derivatives of P1.
Formation of the Tpy-metal (M-Tpy) complexes is easily detectable for all metallopolymer networks due to the strong marker band situated at around 1030 cm −1 , that is selective to M-Tpy moieties. For the formation of Triaz-Py metal complexes (M-Triaz-Py), the confirmation of the selection is less trivial due to the highly overlapping features in the region around 1000 cm −1 . The marker band at ca. 1000 cm −1 for M-Triaz-Py coincides with the band for unbound Tpy, which obfuscates its presence. Nevertheless, the presence of a band at 1000 cm −1 after addition of the metal salts is a clear indicator that Triaz-Py is bound to a metal. For the model polymers P2 (containing only Tpy) as well as in previous studies [37], it was found that the band completely vanishes upon formation of the M-Tpy complexes. Therefore, the remaining intensity at this position can be attributed to the formation of M-Triaz-Py. This confirms the successful formation of a Tpy as well as a Triaz-Py metal complexes in all metallopolymer networks of P1.
Furthermore, for the mixed networks P1-Fe/Zn and P1-Co/Zn, the region between 1500 and 1650 cm −1 (Figure 1, right panel) is also of interest. As mentioned above, the changes to the Raman signature of Triaz-Py are much more pronounced for zinc compared to iron and cobalt here. Indeed, an additional band at ca. 1570 cm −1 can be seen for the metallopolymer networks, indicating successful formation of specifically the Zn-Triaz-Py complexes inside the polymers. This proves the selective complexation of both metal salts to the respective moieties, necessary for the triple shape-memory behavior.

Investigation of the Thermal Properties
To investigate the thermal properties, which represent key parameters for thermal triggered shape-memory process, differential scanning calorimetry (DSC) measurements and thermogravimetric analysis (TGA) were carried out with the synthesized polymer and metallopolymer networks. The results are summarized and displayed in Table 3 as well as Figure 2 (further information in the Supplementary Information Figures S14-S17).
Within the TGA investigation, it is possible to determine the degradation temperature (T d ). This value is important to find out up to what temperature the polymer can be switched without being decomposed. All covalently crosslinked metallopolymer networks P1-Fe/Fe, P1-Co/Co, P1-Fe/Zn, and P1-Co/Zn revealed degradation temperatures above 200 • C enabling the switching based on the more stable terpyridine complex at high temperatures. Table 3. Determined degradation and glass transition temperatures of the polymer network P1 and the corresponding metallopolymer networks P1-Fe/Fe, P1-Co/Co, P1-Fe/Zn, and P1-Fe/Co via thermogravimetric analysis and differential scanning calorimetry.  Furthermore, within the DSC investigation, it was possible to determine the glass transition temperature (T g ) of all samples. Above this temperature, the material becomes soft and flexible enough to be deformed. It turned out that the metallopolymer networks synthesized do not reveal a sharp T g , but rather show a broad area in which they soften (see Table 3) unlike what was found for the polymer P1, which presumably goes in hand with the activation of the metal complexes (see Supplementary Information Figure S14). The measurements revealed the lowest range of softening for the sample P1-Fe/Fe while the highest range was determined for the sample P1-Fe/Zn. The samples P1-Co/Co and P1-Co/Zn revealed relatively comparable softening ranges in the DSC investigations, even though the turnover point for the sample P1-Co/Co was, at 114 • C, slightly higher compared to the value of 101 • C, determined for sample P1-Co/Zn. Nevertheless, all four samples showed a softening in comparable ranges.

Investigation of the Shape-Memory Abilities
In order to investigate the shape-memory abilities of the synthesized covalently crosslinked metallopolymer networks, a permanent shape had to be determined. This was performed analogous to a literature procedure [14]. For this reason, the samples P1-Fe/Fe, P1-Co/Co, P1-Fe/Zn, and P1-Co/Zn were filled into a self-manufactured mold and hot pressed at a temperature of about 150 to 160 • C and a weight of about 1 to 4 t. In this way, a rectangular specimen could be obtained for each sample (exemplarily, see Figure 3a). All synthesized covalently crosslinked metallopolymer networks showed triple shape-memory behavior during a manually performed test. A photo series of the sample P1-Co/Zn is exemplarily presented in Figure 3. For the remaining three samples, it is displayed in the Supplementary Information Figures S31-S33. In the beginning of this test, the sample was heated to 140 • C, a temperature above the activation temperature of both complexes. At this temperature, the sample was elongated and cooled below the activation temperature of the terpyridine complex to fix the first temporary shape (see Figure 3b) via the supramolecular crosslinking of the deactivation of terpyridine complexes. Furthermore, the sample was twisted at a temperature of 80 • C, at which only the triazole-pyridine complexes should be activated, and afterwards cooled to room temperature to determine the second temporary shape (see Figure 3c), fixed by the reformed and non-activated triazole-pyridine complexes. The metallopolymer network stayed in this elongated and twisted shape until it was again heated to 80 • C, leading to the recovery of the temporary shape A (see Figure 3d), by activating the weaker supramolecular crosslinking. Heating the polymer afterwards again to the initial temperature of 140 • C, at which the terpyridine complexes are activated again, induced the restoration of the original permanent shape under shrinking of the metallopolymer network (see Figure 3e). Furthermore, to quantify the shape-memory ability and to compare the different metallopolymer networks with each other, thermo-mechanical analyses (TMA) were performed. Within those measurements it is possible to calculate the strain fixity (R f ) and strain recovery rates (R r ) according to Equations (1) and (2). During this measurement, the sample in its permanent shape (γ A ) was deformed (γ B,load ) above the switching temperature (T sw ) followed by a cooling step below T sw . Afterwards, the stress was completely removed from the sample leading to the fixed temporary shape (γ B ). Heating the sample again to the initial temperature leads to the recovered permanent shape (γ A,rec ). While the strain recovery rate quantifies the ability of the material to fix a mechanical deformation, the strain recovery rate gives information about the quality of the restorage of the original shape.
In the beginning, for each metallopolymer network, standard TMA measurements at two or three switching temperatures were performed to investigate the dual shapememory abilities of the materials at those temperatures. Exemplarily, the two resulting TMA-plots of the sample P1-Fe/Fe are displayed in Figure 4a. All results of this investigation are presented in the Supplementary Information Table S4 and Figures S18-S25. Furthermore, the calculated strain fixity and recovery rates are reported in Table 4. Additionally, the triple shape-memory abilities were also investigated via TMA measurements. Exemplarily, the resulting TMA plot is displayed in Figure 4b for the sample P1-Fe/Fe. The remaining plots are presented in the Supplementary Information (Figures S26-S30). In the beginning, the sample in its permanent shape (γ A ) was heated to the first switching temperature (T sw1 = 150 • C) which was above the activation temperature of the more stable terpyridine complexes. At this temperature, the sample was twisted to determine the first temporary shape (γ B,load ) followed by a cooling step to the second switching temperature (T sw2 = 110 • C or 100 • C). Afterwards, the shear stress was completely removed from the sample followed by an annealing step to determine the fixed first temporary shape (γ B ). The sample was then deformed again, now at the lower temperature of 110 • C, respectively 100 • C, to program the second temporary shape (γ C,load ). Cooling the sample afterwards to 30 • C, releasing the shear stress from the sample and annealing it, leads to the second fixed temporary shape (γ C ). To investigate the regeneration of the different shapes, the sample was heated again under stress free conditions, to firstly 110 • C or 100 • C inducing the recovery of the first temporary shape (γ B,rec ), and afterwards to the initial temperature of 150 • C leading to the regeneration of the original permanent shape (γ A,rec ). With Equations (3)-(8), it is possible to calculate the strain fixity and recovery rates for the single steps as well as the overall values which are summarized in Table 4.  Table 4. Calculated fixity and recovery rates of the metallopolymer networks P1-Fe/Fe, P1-Co/Co, P1-Fe/Zn, and P1-Fe/Co via thermo-mechanical analyses for the investigation of the dual and triple shape-memory abilities.

Investigation of the Dual Shape-Memory Properties
Investigation of the Triple Shape-Memory Properties Fixity Rates (%) Recovery Rates (%) The measurements revealed a moderate strain fixity rate (70 to 87%) for the fixation of the first temporary shape at 110 • C. This is possibly due to the fact that the terpyridine complexes are not yet completely deactivated at this temperature and that the determined form is therefore not completely fixed. The samples containing two different salts (P1-Fe/Zn and P1-Fe/Co) revealed herein higher fixity rates compared to P1-Fe/Fe and P1-Co/Co, which contain only one metal salt. Presumably, the utilization of two different metal salts for the synthesis results in a better deactivation of the terpyridine complex at 110 • C. The current working hypothesis is that for the samples containing the same salt in both complexes, either mixed complexes might be formed as intermediates at 110 • C during the exchange reaction of both metal complexes or different superstructures and morphologies are present due to the different metal ions utilized. The kind of the switching unit seems to influence the reversible behavior of the stable phase (although this is the same for the compared polymers). A similar behavior could already be shown for a different ligand system [37].
Nevertheless, the calculated values of R f1 are quite good for triple shape-memory polymers. In order to investigate whether a reduction in temperature could counteract this phenomenon and, therefore, increase the fixity rate (R f1 ), an additional measurement was carried out with the samples P1-Fe/Fe and P1-Co/Co, in which T sw2 was reduced from 110 to 100 • C. As expected, the fixity rate of this step could be significantly increased. The fixation of the second temporary shape was excellent for all samples within a calculated strain fixity rate for this step of 100%. Furthermore, the calculated recovery rates of the samples showed satisfying results. For the measurement performed with T sw2 = 110 • C, the best performing sample regarding the recovery rates was P1-Fe/Fe, which revealed R r values of about 95% for both recovery steps. Moreover, the sample P1-Co/Co revealed good recovery behavior, in particular during the first recovery step. This is exactly the opposite behavior to the first fixation step. The fact that these two samples fixed worse in the first step seems to in turn improve the recovery behavior, which presumably results from the behavior described above. Matching this, the reduction of T sw2 to 100 • C also reduced the calculated value for R r1 . It has to be noted that during the second recovery step for the sample P1-Co/Zn and P1-Co/Co (at T sw2 = 100 • C), a recovery rate above 100% (R f2 = 109.4%, respectively 104.2%) was found. This can be explained by an incomplete recovery during the first recovery step, which is often noticed during the characterization of triple shape-memory polymers [23,33,40]. The sample P1-Fe/Zn in general revealed, compared to the other three samples, the lowest recovery rates which may have resulted from its thermal properties. Looking at the previous DSC investigations, it becomes clear that this sample has the highest T g . Therefore, this sample can be considered as less soft as the other three polymer networks resulting in a lower recovery. Nevertheless, these lower recovery rates above 83% are still within a good range if compared to values from the literature for other triple shape-memory polymer systems.
In literature, there are several examples for triple and even multiple shape-memory polymers [23,32,40,41]. However, a system that is very similar in structure to the herein presented triple shape-memory metallopolymer networks, in which both temporary forms can be switched via two different reversible supramolecular metal-ligand interactions, is to the best of our knowledge not available. Comparable reports describe polymers featuring supramolecular crosslinks via hydrogen bonds. These materials exhibit good triple shapememory abilities [32]. Another example is the utilization of side chain liquid crystallization for the creation of triple SMPs. The TMA investigation of this kind of material revealed comparable results, with R f1 values from 56 to 79%, R f2 values near 100% and recovery rates similar to those of the presented metallopolymer networks [40]. Overall, the synthesized covalently crosslinked metallopolymer networks P1-Fe/Fe, P1-Co/Co, P1-Fe/Zn, and P1-Co/Zn revealed comparable shape-memory properties to other triple shape-memory polymers known from literature.

Conclusions
In the scope of this study, we were able to successfully synthesize triple shape-memory metallopolymer networks in which the switching of the two temporary shapes could be realized by activating and deactivating metal-ligand interactions of different stability. The synthesized materials were analyzed in a detailed fashion. Thermogravimetric analyses and differential scanning calorimetry were utilized to investigate the thermal properties. Additionally, within isothermal titration calorimetry and FT-Raman spectroscopy, it was possible to investigate the different metal-ligand interactions utilized for the reversible crosslinking. The performed thermo-mechanical analyses revealed very good dual and triple shape-memory abilities for all synthesized metallopolymer networks. Results showed that the sample P1-Fe/Fe is the best performer during the recovery step (both recovery rates above 95%). In contrast, the samples containing two different salts P1-Fe/Zn and P1-Co/Zn revealed the highest strain fixity rates for the first fixation step. In summary, the presented metallopolymer networks exhibit a good triple shape-memory performance.